3D Printing/Vat Photopolymerization of Photopolymers Activated by Novel Organic Dyes as Photoinitiators

: Even though numerous organic dyes which are used as photoinitiators/photocatalysts during photopolymerization have been systematically investigated and collected in previous reviews, further designs of these chromophores and the developments in high-performance photoinitiating systems have emerged in recent years, which play the crucial role in 3D printing/Vat polymerization. Here, in this mini-review, various families of organic dyes that are used as newly synthesized photoinitiators/photocatalysts which were reported in literature during 2021–2022 are speciﬁed by their photoinitiation mechanisms, which dominate their performance during photopolymerization, especially in 3D printing. Markedly, visible light-induced polymerization could be employed in circumstances not only upon the irradiation of artiﬁcial light sources, e.g., in LEDs, but also in sunlight irradiation. Furthermore, a short overview of the achievements of newly developed mechanisms, e.g., RAFT, photoinitiator-RAFT, and aqueous RAFT using organic chromophores as light-harvesting compounds to induce photopolymerization upon visible light irradiation are also thoroughly discussed. Finally, the reports on the semiconducting nanomaterials that have been used as photoinitiators/photocatalysts during photopolymerization are also introduced as perspectives that are able to expand the scope of 3D printing and materials science due to their various advantages such as high extinction coefﬁcients, broad absorption spectra, and having multiple molecular binding points.


Introduction
Nowadays, 3D printing/vat photopolymerization, namely additive manufacturing, has been widely known as a powerful tool in rapid prototype design and in the production of three-dimensional objects [1][2][3]. Indeed, a number of 3D objects have been successively prototyped in academic laboratories around the world, remarkably, the photopolymerization process has already found an uncontested place in the stereolithography technique or in 3D printing [4][5][6]. This approach provides an efficient way to solidify liquid resins into designed objects under light irradiation, among various 3D printing technologies [7][8][9]. Moreover, photopolymerization is also regarded as an emerging technique for many other fields, e.g., (i) regenerative medicine and photocurable dental composites [10,11], (ii) drug delivery [12], and (iii) 4D printing [13,14]. In particular, Light Emitted Diodes (LEDs) with a safe amount of violet light were widely used as a reliable artificial light sources to activate the polymerization process by a number of research groups due to them having numerous advantages such as a low-cost, spatial control, a highly efficient process in mild conditions, and being safe [4,15]. Obviously, the wavelength and intensity of the light source affect the performance of the polymerization process [16,17]. On the other hand, sunlight is a natural light source that tends to be more widely used for photopolymerization in the laboratory (TMPTA). Remarkably, NPIE1 exhibited a better photoinitiation ability than the benchmark PI diphenyl (2,4,6-trimethyl-benzoyl)phosphine oxide (TPO) did in both of the cases of 405 and 455 nm irradiation (final conversion of TPO: 66% @405nm LED, no polymerization @455 nm LED). In addition, a decarboxylation reaction was also detected, thus the mechanisms of Type I PI that occurred during the polymerization process can be imagined. Finally, a high thermal stability of the investigated NPIEs in the acrylate monomers was found, and their good photoinitiation abilities were also verified by the success of the 3D printing experiments [48].

Bis-chalcones Based Oxime Ester Derivatives
In photochemistry, an oxime ester is also commonly regarded as Type I photoinitiator. Numerous families of oxime esters which are derived from coumarin-carbazole, nitro-carbazole, and phenylthioether thiophene dyes were designed for LED photopolymerization [49][50][51]. In 2022, Wu, X. et al. firstly synthesized three bis-chalcones-based oxime ester dyes (marked as TA1-3), and they used them as Type I PIs to conduct the photopolymerization of an acrylate monomer (1, 6-hexanediol diacrylate, HDDA) under its exposure to a 455 nm LED for 30 min. In this polymerization process, the monomer that was initiated by the TA2 with benzylidene cyclopentanone oxime ester exhibited the highest final conversion (see Table 1) and photoinitiation efficiency owing to its best electron delocalization among the three chromophores. Remarkably, a photobleaching phenomenon was also observed on these dyes with the same concentration (1 × 10 −6 mol·g −1 ) in the HDDA system via the photocuring depth experiment upon its exposure to a 455 nm LED (see Figure 1). The colors of all of the dyes seem to be completely disappeared. Surprisingly, the largest photobleaching height of the columns was achieved by the photopolymerization that was initiated by TA2, reaching the depth of 32mm in thickness (see Figure 1b). Indeed, their photobleaching properties are likely to expand the knowledge of the structural design of the dyes and reveal the potential in deep photocuring and the applications for visible light photoinitiators, e.g., 3D printing and dental materials [52].  Table 2. Among them, three PIs with acetyl (OXE-M), acryloyl . Adapted from [52] with permission from Elsevier. Table 1. Newly developed N-hydroxynaphthalimide esters applicable in PISs as Type I photoinitiators [48,52].

No.
OXEs Absorption Properties Conversion 1 system via the photocuring depth experiment upon its exposure to a 455 nm LED (see Figure 1). The colors of all of the dyes seem to be completely disappeared. Surprisingly, the largest photobleaching height of the columns was achieved by the photopolymerization that was initiated by TA2, reaching the depth of 32mm in thickness (see Figure 1b). Indeed, their photobleaching properties are likely to expand the knowledge of the structural design of the dyes and reveal the potential in deep photocuring and the applications for visible light photoinitiators, e.g., 3D printing and dental materials [52].  The chemical structures  of four investigated dyes (OXE-M, OXE-V, OXE-P, and OXE-H) and their absorption properties are listed in Table 2. Among them, three PIs with acetyl (OXE-M), acryloyl (OXE-V), and benzoyl (OXE-P) terminal groups within the oxime ester group were firstly synthesized. Remarkably, the three PIs exhibited excellent photoinitiation abilities during the photopolymerization of the acrylate monomers (TMPTA) under 405 nm LED irradiation. Specifically, the OXE-M/TMPTA system achieved higher final conversion (~69% for TMPTA) than that of the commercial Type I photoinitiator system ((diphenyl(2,4,6-trimethylbenzoyl) phosphine oxide TPO/TMPTA,~65%) [53]. Table 2. Newly developed oxime esters (OXEs) that are applicable as Type I photoinitiators [53,54].

~56%
In addition, the chemical mechanisms of the OXEs during the polymerization process are proposed and depicted in Figure 2a. Upon their irradiation under a 405 nm LED, the iminyl and acyloxy radicals were generated from the cleavage of the N-O bond, which occurred upon the excitation of the OXE. Subsequently, a highly active free radical (R • ) can be released from the acyloxy radical by a decarboxylation process to promote the polymerization of the acrylate monomers. Finally, the direct laser writing experiments and 3D printing were applied on an OXE-M/TMPTA system to confirm the high reactivity of the proposed PIs in the TMPTA. The letter pattern "OXE" with smooth surfaces and a good spatial resolution was observed as is shown in Figure 2c. Moreover, a square frame was also printed (see Figure 2d) by using a low light intensity 3D printer at 405 nm laser diode (110 mW cm −2 ) under air. Owing to the excellent performances of the nitrocarbazole oxime esters during photopolymerization, they could be ideal Type I photoinitiators for highly efficient 3D printing. Furthermore, the success in preparing the carbon fiber composites with the OXE-M-based system also revealed the dual photo/thermal initiation behaviors of OXE-M since minor light transmission was observed during the preparation process.

6%
In addition, the chemical mechanisms of the OXEs during the polymerization process are proposed and depicted in Figure 2a. Upon their irradiation under a 405 nm LED, the iminyl and acyloxy radicals were generated from the cleavage of the N-O bond, which occurred upon the excitation of the OXE. Subsequently, a highly active free radical (R • ) can be released from the acyloxy radical by a decarboxylation process to promote the polymerization of the acrylate monomers. Finally, the direct laser writing experiments and 3D printing were applied on an OXE-M/TMPTA system to confirm the high reactivity of the proposed PIs in the TMPTA. The letter pattern "OXE" with smooth surfaces and a good spatial resolution was observed as is shown in Figure 2c. Moreover, a square frame was also printed (see Figure 2d) by using a low light intensity 3D printer at 405 nm laser diode (110 mW cm −2 ) under air. Owing to the excellent performances of the nitrocarbazole oxime esters during photopolymerization, they could be ideal Type I photoinitiators for highly efficient 3D printing. Furthermore, the success in preparing the carbon fiber composites with the OXE-M-based system also revealed the dual photo/thermal initiation behaviors of OXE-M since minor light transmission was observed during the preparation process.
In a continuation of the previous research, Liu, S. et al. introduced 50 newly synthesized nitrocarbazole oxime esters with different structures in five series [54]. Ten of these chromophores were systematically investigated, and their light absorption properties and the final conversions (FCs) of the TMPTA in the presence of the OXEs upon their exposure to an LED@405 nm are depicted (which are marked as the numbers [5][6][7][8][9][10][11][12][13][14] in Table 2. In this work, the chromophores with the methyl substituent on the oxime ester group (B1, C1, D1, E1, and F1) exhibited the best performances and photoinitiation ability during the polymerization process owing to their specific structures which allow for the generation of highly reactive radicals. Interestingly, the decarboxylation reactions that occurred more easily in D1 than they did in D2 were observed by establishing a profile of the absorption intensity curves (absorbance vs. irradiation time) to monitor the generation of CO 2 (see Figure 3b). As a result, the decarboxylation reactions that appeared within the first 16s of the photopolymerization process are proven, which promotes the polymerization process. This phenomenon could also be regarded as an important reason why D1 shows better a photoinitiation ability than D2 does upon its exposure to both an LED@405 nm and an LED@365 nm. To certify the excellent photoinitiation capability of the nitrocarbazole oxime ester, the D1/TMPTA system was selected and studied in direct laser writing (DLW) experiments due to its high photoinitiation efficiency at 405 nm. As expected, a letter pattern "ET" (thickness ∼1600 µm, see Figure 3c) and two 3D objects (thickness ∼2 mm) with high spatial resolutions were successfully obtained within a short time (∼2 min) by using a stereolithography 3D printer. In a continuation of the previous research, Liu, S. et al. introduced 50 newly synthesized nitrocarbazole oxime esters with different structures in five series [54]. Ten of these chromophores were systematically investigated, and their light absorption properties and the final conversions (FCs) of the TMPTA in the presence of the OXEs upon their exposure to an LED@405 nm are depicted (which are marked as the numbers [5][6][7][8][9][10][11][12][13][14] in Table 2. In this work, the chromophores with the methyl substituent on the oxime ester group (B1, C1, D1, E1, and F1) exhibited the best performances and photoinitiation ability during the polymerization process owing to their specific structures which allow for the generation of highly reactive radicals. Interestingly, the decarboxylation reactions that occurred more easily in D1 than they did in D2 were observed by establishing a profile of the absorption intensity curves (absorbance vs. irradiation time) to monitor the generation of CO2 (see Figure 3b). As a result, the decarboxylation reactions that appeared within the first 16s of the photopolymerization process are proven, which promotes the polymerization process. This phenomenon could also be regarded as an important reason why D1 shows better a photoinitiation ability than D2 does upon its exposure to both an LED@405 nm and an LED@365 nm. To certify the excellent photoinitiation capability of the nitrocarbazole oxime ester, the D1/TMPTA system was selected and studied in direct laser writing (DLW) experiments due to its high photoinitiation efficiency at 405 nm. As expected, a letter pattern "ET" (thickness ∼1600 μm, see Figure 3c) and two 3D objects (thickness ∼2 mm) with  high spatial resolutions were successfully obtained within a short time (∼2 min) by using a stereolithography 3D printer.   system. Line 2: photopolymerization profiles (acrylate function conversion vs. irradiation time) of the D2/TMPTA system. Line 3: the curve of absorption intensity (absorbance vs. irradiation time) of CO 2 that was obtained from the D1/TMPTA system. Line 4: the curve of absorption intensity (absorbance vs. irradiation time) of CO 2 that was obtained from the D2/TMPTA system. (c) Letter pattern that was observed using a digital microscope. Adapted from [54] with permission from the American Chemistry Society.

Type II Photoinitiators
As it is aforementioned in the text, a wide range of chromophores with different structures have been investigated as reliable Type II photoinitiators to activate free-radical photopolymerization. Remarkably, intense efforts were not only devoted to the development of photopolymerization upon the irradiation of a 405 nm light-emitting diode (LED), but they were also devoted noticeably to sunlight-induced photopolymerization [18][19][20], which is introduced in the following context. Similar to the mechanisms that are shown in Equations (2)-(4), the reactions that occurred in the dye-based three-component systems (dye/co-PI/additive) during the free-radical polymerization processes can be supported by two existing interactions between the dye/co-PI and the dye/additive (Equations (7)-(11), photoinitiation mechanisms of dyes/Iodonium/amine redox combination [33,37]). Indeed, the reaction mechanisms of the Type II photoinitiatiator/photocatalyst have been introduced in the previous literature, precisely and systematically [33,37].

Benzophenone Derivatives
Benzophenone derivatives are commonly used as Type II photoinitiators after the chemical modifications of them have been performed by moieties such as triphenylamine [55], carbazole [56], stilbene [57], and naphthalimide [58]. As possible hydrogen acceptors, benzophenone derivatives are often paired with other co-initiators acting as hydrogen donors to proceed with the electron/proton transfer. However, they have also been used in a onecomponent photoinitiating system (PIS) to initiate photopolymerization efficiently [26,59].
Recently, Huang, T. synthesized five benzophenone derivatives (BPN-D, BPN-P, BPN-N, BPN-An, and BPN-Py) by chemically modifying benzophenone with a tertiary amine, and they used them as one-component PISs during the photopolymerization of trimethylolpropane trimethacrylate (TMPTMA) under the irradiation both of a UV lamp and a 405 nm LED. Here, the light absorption properties of benzophenone derivatives (which are noted as dyes 1-5) and the conversions of the acrylates are summarized in Table 3. From the results, the highest acrylate conversion that occurred under the UV lamp irradiation could be observed when BPN-Ph acted as a photoinitiator (FC~30%), while the highest conversion under the 405 nm LED irradiation was achieved by using BPN-An as photoinitiator (FC~22%). After comparing them with the commercial analogs, 4-(diethylamino) benzophenone (BPN), and 4,4 -bis(diethylamino) benzophenone (EMK), the newly synthesized derivatives were regarded as efficient Type I photoinitiators with enhanced photosensitivity, organic solubility, and optical and thermal properties during the photopolymerization process [60]. Table 3. Newly developed benzophenone derivatives that are applicable as Type II photoinitiators [60,61].

Organic Dyes Absorption Properties Conversion (Monomer
On the other hand, the dye-based PISs with benzophenone derivatives can not only be used to initiate free-radical photopolymerization (FRP), but they can also be used to initiate cationic photopolymerization (CP). In 2021, Liu et al. synthesized seven new chro- On the other hand, the dye-based PISs with benzophenone derivatives can not only be used to initiate free-radical photopolymerization (FRP), but they can also be used to initiate cationic photopolymerization (CP). In 2021, Liu et al. synthesized seven new chromophoroes with benzophenone moieties as Type II photoinitiators for photopolymeriza- On the other hand, the dye-based PISs with benzophenone derivatives can not only be used to initiate free-radical photopolymerization (FRP), but they can also be used to initiate cationic photopolymerization (CP). In 2021, Liu et al. synthesized seven new chromophoroes with benzophenone moieties as Type II photoinitiators for photopolymerization upon their irradiation under a 405 nm LED. Precisely, the investigated dyes could be On the other hand, the dye-based PISs with benzophenone derivatives can not only be used to initiate free-radical photopolymerization (FRP), but they can also be used to initiate cationic photopolymerization (CP). In 2021, Liu et al. synthesized seven new chromophoroes with benzophenone moieties as Type II photoinitiators for photopolymerization upon their irradiation under a 405 nm LED. Precisely, the investigated dyes could be BC-3 λ max~4 09 nm ε max~2 6,700 M −1 cm −1 ε 405nm~2 6,500 M −1 cm −1~7 0% in TMPTÃ 38% in EPOX On the other hand, the dye-based PISs with benzophenone derivatives can not only be used to initiate free-radical photopolymerization (FRP), but they can also be used to initiate cationic photopolymerization (CP). In 2021, Liu et al. synthesized seven new chromophoroes with benzophenone moieties as Type II photoinitiators for photopolymerization upon their irradiation under a 405 nm LED. Precisely, the investigated dyes could be divided into two series by their functional groups, (1) the dyes with benzophenonetriphenylamine hybrid structures (which are noted as BT1-BT4) and (2) the dyes with benzophenone-carbazole hybrid structures (which are noted as BC1-BC3). Markedly, their specific chemical structures contribute to the red-shift of the absorption maxima and the enhancement of their molar extinction coefficients (see Table 3, dyes 6-12). In this work, all of the one-component PISs (the dyes alone), two-component PISs (dye/Iod or dye/EDB), and three-component PISs (dye/Iod/EDB) were investigated for photopolymerization upon their irradiation with a 405 nm LED. The polymerization profiles are presented in Figure 4, and the final function conversions (FCs) were collected, and they are presented in Table 3. In terms of the results, all of the benzophenone derivatives could initiate the photopolymerization of the TMPTA, either in one-(dye alone), two-(dye/Iod or dye/EDB), or three-component (dye/Iod/EDB) PISs. (see Figure 4a,b (or c),d, respectively). Remarkably, better hydrogen abstraction abilities were found for the benzophenone-triphenylamine derivatives, BT2, BT3, and BT4, rather than the commercial photoinitiator, 2-isopropylthioxanthone. Among them, BT3, with a high molecular weight, trifunctional character, and excellent migration stability, was applied in 3D printing and good 3D patterns were attained [61].  Figure 4a,b (or c),d, respectively). Remarkably, better hydrogen abstraction abilities were found for the benzophenone-triphenylamine derivatives, BT2, BT3, and BT4, rather than the commercial photoinitiator, 2-isopropylthioxanthone. Among them, BT3, with a high molecular weight, trifunctional character, and excellent migration stability, was applied in 3D printing and good 3D patterns were attained [61]. Previously, a wide range of push-pull dyes have been investigated as reliable photoinitiators (PIs) to activate free-radical photopolymerization [18][19][20]34]. In the previous research, the photoinitiation capabilities of two series of push-pull dye-based three-com- The photopolymerization starts at t = 10 s. Adapted from [61] with permission from the Royal Society of Chemistry and the Chinese Chemical Society.
In 2022, a series of indane-1,3-dione and 1H-cyclopenta[b]naphthalene-1,3(2H)-dione derivatives (which are noted as dyes 1-13) were initially synthesized by Sun, K. et al., and then, the photopolymerization of the benchmark acrylate monomer (TMPTA) which was initiated by the dyes 1-13-based three-component PISs was also examined by RT-FTIR experiments upon their irradiation with a 405 nm LED at room temperature. The photopolymerization profiles and conversions of the TMPTA are presented in Figure 5a and Table 4, respectively. Among them, the final acrylate conversions of the TMPTA that were obtained in the presence of the dyes 7, 9, and 11-based PISs (≈97-99%) were markedly higher than those of the reference system (Iod/EDB combination without dye, noted dye 0, FC~60%). Moreover, the efficient dyes 7, 9, and 11-based systems were selected to activate the sunlight-induced photopolymerizations of the TMPTA. As expected, the three selected dyes produced high FCs in 30 min of sunlight irradiation, (FC~99% for dye 7, FC~95% for dye 9, and FC~92% for dye 11, see Table 4 and Figure 5b), which again certified the outstanding photoinitiation abilities of the indane-1,3-dione and 1H-cyclopenta[b] naphthalene-1,3(2H)-dione derivatives and their potential use as efficient light-harvesting compounds, both under artificial and natural light sources [62].

4-dimethoxyphenyl-1-allylidene Derivatives
As an additional piece of research on the N-ethylcarbazole-1-allylidene derivatives, 12 derivatives with substitutions of the 4-dimethoxyphenyl-1-allylidene groups were examined for their use as three-component PISs. Similarly, they exhibited outstanding photochemical properties and chemical reactivity in promoting the FRP processes. Here, Table 5 summarizes their photochemical properties, chemical structures, absorption properties, and the final conversions of the monomer that was under initiation is listed as follows after referring to the published review and literature [37,62].
Combining with the results achieved from the family of N-ethylcarbazole-1-allylidene derivatives mentioned above, sunlight is proved repeatedly to be a reliable natural light source for free-radical polymerization, and the group of push-pull dyes with high photoinitiation abilities upon sunlight irradiation is expanded as well. In Sun's work, the Direct Laser Writing/3D printing experiments were also applied to the three-component PISs using the indane-1,3-dione, 1H-cyclopenta[b]naphthalene-1,3(2H)-dione derivatives. After the printing process, the 3D patterns were successfully fabricated using the all of the chosen dye-based three-component PISs with/without silica powders as fillers in an acrylate monomer (TMPTA). As shown in Figure 6, the 3D profiles with smooth surfaces and excellent spatial resolutions were profilometrically observed by numerical optical microscopy ("LZ" for dye 7, "CD" for dye 9, "YR" for dye 11, "RUY" for dye 7/silica, "SAQ" for dye 9/silica, and "HUI" for dye 11/silica), thereby giving powerful support to the truth that the dyes with indane-1,3-dione, 1H-cyclopenta[b]naphthalene-1,3(2H)-dione can be regarded as reliable Type II photinitiators with a high light ab-  then, the photopolymerization of the benchmark acrylate monomer (TMPTA) which was initiated by the dyes 1-13-based three-component PISs was also examined by RT-FTIR experiments upon their irradiation with a 405 nm LED at room temperature. The photopolymerization profiles and conversions of the TMPTA are presented in Figure 5a and Table 4, respectively. Among them, the final acrylate conversions of the TMPTA that were obtained in the presence of the dyes 7, 9, and 11-based PISs (≈97-99%) were markedly higher than those of the reference system (Iod/EDB combination without dye, noted dye 0, FC~60%). Moreover, the efficient dyes 7, 9, and 11-based systems were selected to activate the sunlight-induced photopolymerizations of the TMPTA. As expected, the three selected dyes produced high FCs in 30 min of sunlight irradiation, (FC~99% for dye 7, FC~95% for dye 9, and FC~92% for dye 11, see Table 4 and Figure 5b), which again certified the outstanding photoinitiation abilities of the indane-1,3-dione and 1H-cyclopenta[b] naphthalene-1,3(2H)-dione derivatives and their potential use as efficient lightharvesting compounds, both under artificial and natural light sources [62].

4-dimethoxyphenyl-1-allylidene Derivatives
As an additional piece of research on the N-ethylcarbazole-1-allylidene derivatives, 12 derivatives with substitutions of the 4-dimethoxyphenyl-1-allylidene groups were examined for their use as three-component PISs. Similarly, they exhibited outstanding photochemical properties and chemical reactivity in promoting the FRP processes. Here, Table 5 summarizes their photochemical properties, chemical structures, absorption properties, and the final conversions of the monomer that was under initiation is listed as follows after referring to the published review and literature [37,62].

4-dimethoxyphenyl-1-allylidene Derivatives
As an additional piece of research on the N-ethylcarbazole-1-allylidene derivatives, 12 derivatives with substitutions of the 4-dimethoxyphenyl-1-allylidene groups were examined for their use as three-component PISs. Similarly, they exhibited outstanding photochemical properties and chemical reactivity in promoting the FRP processes. Here, Table 5 summarizes their photochemical properties, chemical structures, absorption properties, and the final conversions of the monomer that was under initiation is listed as follows after referring to the published review and literature [37,62].

4-dimethoxyphenyl-1-allylidene Derivatives
As an additional piece of research on the N-ethylcarbazole-1-allylidene derivatives, 12 derivatives with substitutions of the 4-dimethoxyphenyl-1-allylidene groups were examined for their use as three-component PISs. Similarly, they exhibited outstanding photochemical properties and chemical reactivity in promoting the FRP processes. Here, Table 5 summarizes their photochemical properties, chemical structures, absorption properties, and the final conversions of the monomer that was under initiation is listed as follows after referring to the published review and literature [37,62].
Combining with the results achieved from the family of N-ethylcarbazole-1-allylidene derivatives mentioned above, sunlight is proved repeatedly to be a reliable natural light source for free-radical polymerization, and the group of push-pull dyes with high photoinitiation abilities upon sunlight irradiation is expanded as well.
Combining with the results achieved from the family of N-ethylcarbazole-1-allylidene derivatives mentioned above, sunlight is proved repeatedly to be a reliable natural light source for free-radical polymerization, and the group of push-pull dyes with high photoinitiation abilities upon sunlight irradiation is expanded as well.
Combining with the results achieved from the family of N-ethylcarbazole-1-allylidene derivatives mentioned above, sunlight is proved repeatedly to be a reliable natural light source for free-radical polymerization, and the group of push-pull dyes with high photoinitiation abilities upon sunlight irradiation is expanded as well.
Combining with the results achieved from the family of N-ethylcarbazole-1-allylidene derivatives mentioned above, sunlight is proved repeatedly to be a reliable natural light source for free-radical polymerization, and the group of push-pull dyes with high photoinitiation abilities upon sunlight irradiation is expanded as well. 9% @405 nm LED In Sun's work, the Direct Laser Writing/3D printing experiments were also applied to the three-component PISs using the indane-1,3-dione, 1H-cyclopenta[b]naphthalene-1,3(2H)-dione derivatives. After the printing process, the 3D patterns were successfully fabricated using the all of the chosen dye-based three-component PISs with/without silica powders as fillers in an acrylate monomer (TMPTA). As shown in Figure 6, the 3D profiles with smooth surfaces and excellent spatial resolutions were profilometrically observed by numerical optical microscopy ("LZ" for dye 7, "CD" for dye 9, "YR" for dye 11, "RUY" for dye 7/silica, "SAQ" for dye 9/silica, and "HUI" for dye 11/silica), thereby giving powerful support to the truth that the dyes with indane-1,3-dione, 1Hcyclopenta[b]naphthalene-1,3(2H)-dione can be regarded as reliable Type II photinitiators with a high light absorption capacity and excellent photoinitiation abilities in FRP. As a conclusion, the photocomposites that were attained in the presence of silica fillers are able to be utilized as useful photochemical materials in the fields of additive manufacturing/vat photopolymerization, etc.

Mechanisms of Newly Developed Photo-Reversible Deactivation Radical Polymerization (Photo-RDRP Polymerization) and Their Applications in 3D Printing
Although the basic mechanisms of the free-radical polymerization that is mentioned above have been systematically discussed and applied in the synthesis of polymer networks and 3D printing, another radical polymerization mechanism that is called reversible deactivation radical polymerization (RDRP) is also well adopted. It can be further categorized into four classes: 1.nitroxide-mediated polymerization (NMP), 2. photoiniferter polymerization (mechanisms shown as Figure 7a), 3. atom transfer radical polymerization (ATRP, mechanisms shown as Figure 7b), and 4. reversible addition-fragmentation chain transfer polymerization (RAFT, mechanisms shown as Figure 7c). Interestingly, they offer stronger capabilities to control the polymer architectures and propagate dormant reactivatable species than the conventional polymerization process does [63]. Inspired by the traditional RDRP systems that use thermal initiators to generate active radicals, the photo-RDRPs have been designed to form active radicals and promote chain extension due to the light stimulus. In particular, photoinduced reversible addition-fragmentation chain transfer polymerization (photo-RAFT) has been widely used in numerous fields as an efficient switchable polymerization technique owing to its easy operational process and high tolerance to solvents and monomer functional groups. Specifically, a photoinduced electron/energy transfer (PET) mechanism is commonly adopted to regulate the polymerization process [27,[64][65][66][67]. The generation of active radicals can be repeated by the electron or the energy transfer between the excited catalyst and a RAFT agent under the light irradiation condition. Markedly, if we introduce the advantages of RAFT polymerization into photocured 3D printing, e.g., stereolithography (SLA) and digital light projection (DLA), an efficient RAFT polymerization system that is activated by light will be a crucial factor to allow accurate printing and fast building speeds to be achieved. Four-dimensional printing with the RAFT polymerization technique is also possible with a further modification of the basis of 3D printing [68].

Mechanisms of Newly Developed Photo-Reversible Deactivation Radical Polymerization (Photo-RDRP Polymerization) and Their Applications in 3D Printing
Although the basic mechanisms of the free-radical polymerization that is mentioned above have been systematically discussed and applied in the synthesis of polymer networks and 3D printing, another radical polymerization mechanism that is called reversible deactivation radical polymerization (RDRP) is also well adopted. It can be further categorized into four classes: 1.nitroxide-mediated polymerization (NMP), 2. photoiniferter polymerization (mechanisms shown as Figure 7a), 3. atom transfer radical polymerization (ATRP, mechanisms shown as Figure 7b), and 4. reversible addition-fragmentation chain transfer polymerization (RAFT, mechanisms shown as Figure 7c). Interestingly, they offer stronger capabilities to control the polymer architectures and propagate dormant reactivatable species than the conventional polymerization process does [63]. Inspired by the traditional RDRP systems that use thermal initiators to generate active radicals, the photo-RDRPs have been designed to form active radicals and promote chain extension due to the light stimulus. In particular, photoinduced reversible addition-fragmentation chain transfer polymerization (photo-RAFT) has been widely used in numerous fields as an efficient switchable polymerization technique owing to its easy operational process and high tolerance to solvents and monomer functional groups. Specifically, a photoinduced electron/energy transfer (PET) mechanism is commonly adopted to regulate the polymerization process [27,[64][65][66][67]. The generation of active radicals can be repeated by the electron or the energy transfer between the excited catalyst and a RAFT agent under the light irradiation condition. Markedly, if we introduce the advantages of RAFT polymerization into photocured 3D printing, e.g., stereolithography (SLA) and digital light projection (DLA), an efficient RAFT polymerization system that is activated by light will be a crucial factor to allow accurate printing and fast building speeds to be achieved. Four-dimensional printing with the RAFT polymerization technique is also possible with a further modification of the basis of 3D printing [68].  Even if some attempts using the organic dye/initiator-mediated systems have been performed in RAFT polymerization to print well-defined objects, these photo-RAFT polymerization systems are considered to be used in the cases when very high concentrations of divinyl monomers exist ([crosslinker]:[monomer] > 70:30). In 2021, Lee, K. et al. reported using a photoinitiator-RAFT system containing diphenyl (2,4,6-trimethylbenzoyl) phosphine oxide (TPO) and 2-(n-butylthiocarbonothioylthio) propanoic acid (BTPA) as a Norrish Type I photoinitiator and RAFT agent, respectively, to conduct a RAFT polymerization on two acrylate monomers (N,N-dimethylacrylamide, DMAm, and a poly(ethylene glycol) diacrylate, PEGDA, which was used as crosslinker). Surprisingly, a complicated 3D Eiffel Tower arch was obtained with good resolution and fine details at a rapid printing speed (2.1 cm h −1 ) under 405 nm of violet light irradiation by using a low concentration of crosslinker, where the ratio was set as [PEGDA]:[DMAm] = 40:160 in the presence of BTPA and TPO, respectively (see Figure 8). Specifically, with the use of the photoinitiator-RAFT system, no significant difference in the layer shrinkage was found

Oxygen-Tolerant Reversible Addition-Fragmentation Chain Transfer Polymerization (Oxygen Tolerant RAFT Polymerization)
In the light-induced RDRP, deoxygenation is essential to avoid the occurrence of uncontrolled polymerization since the existing oxygen may interact with the initiation of the radicals during the polymerization process. Thus, an oxygen-tolerant RAFT polymerization was carried out in the early works to prevent the oxygen inhibition during polymerization that happened in a complex system. In the previous research, some methods such as freeze-pump-thaw cycles, inert gas bubbling, and the use of reducing agents in the activators were commonly utilized to remove the oxygen, and some industrial applications of oxygen-tolerant RAFT polymerization were achieved successfully [70][71][72][73]. Alternatively, the possibility of efficiently preventing oxygen inhibition in open air by using photoredox catalysts or other additives has been proved. For instance, a previous enzyme strategy by Enciso, A. E. et al. which used glucose oxidase (GO x ) was reported to deoxygenate and initiate the polymerization process [74].
Recently, Huang Y. et al. developed a simple and green method for oxygen-tolerant RAFT polymerization to occur under aqueous conditions in the open air. In this work, only 4-cyanopentanoic acid dithiobenzoate (CPADB) was used as an intrinsic photoredox catalyst to generate the dithioester anions without the use of another photocatalyst/photoinitiator. In detail, the generated dithioester anions could be stabilized by the amine radical cations that were released from a self-catalyzing monomer, 2-(dimethylamino) ethylmethacrylate (DMAEMA), as an electron donor. Specifically, the mechanisms of the deoxygenation process that occur during photopolymerization are shown in Figure 9. In terms of the results, the photoinduced RAFT polymerization of the mixture in the ratio of [DMAEMA] 0 :[CPADB] 0 = 400:1 during a flame-sealing process without prior deoxygenation successfully proceeded in a controlled fashion, and it produced a high conversion rate of 75% after 24 h. Remarkably, the monomer conversions also increased with the molecular weight and viscosity, proving the fact that dithioester can be used as an iniferter agent to conduct RAFT polymerization under light irradiation. Interestingly, the polymerization in this work was carried out under a simple light source from a household lamp ( As a non-toxic, cheap, and environmentally friendly solvent, water also can be utilized for photopolymerizations to replace the organic solvents that are used in the traditional method. Combined with the advantages of RAFT polymerization, aqueous RAFT Figure 9. Proposed mechanism of oxygen-tolerant RAFT polymerization using dithioester as a photoredox catalyst and amine monomer as an electron donor. []*: excited state of photoredox catalyst. Adapted from Reference [75] with permission from the European Chemical Societies.

Light-Induced Aqueous Reversible Addition-Fragmentation Chain Transfer Polymerization (Aqueous Photo-RAFT Polymerization)
As a non-toxic, cheap, and environmentally friendly solvent, water also can be utilized for photopolymerizations to replace the organic solvents that are used in the traditional method. Combined with the advantages of RAFT polymerization, aqueous RAFT can be potentially applied for many applications due to its benefits, such as the spatiotemporal control of the polymerization process by turning the light source on/off [76]. Commonly, aqueous RAFT photopolymerization is separated into three main categories: one that is catalyzed by the external photoinitiators, e.g., sodium phenyl-2,4,6-trimethylbenzoyl phosphinate (SPTP) and (2,4,6-Trimethylbenzoyl)diphenylphosphine oxide (TPO) [77], one that is catalyst free (photoiniferter) [78], and the aqueous PET-RAFT one [79]. Moreover, aqueous RAFT polymerization can be integrated with other fields to produce functional materials. For instance, McClelland et al. introduced the nanoparticles, e.g., CdSe quantum dots which are used as photocatalysts that can be easily separated and recycled from the polymer product for the aqueous photo-RAFT polymerization [80]. Nowadays, many organic/inorganic chemicals were designed to catalyze the RAFT photopolymerization in the water as a reliable polymerization solvent, and these significantly expanded the applications of aqueous RAFT polymerization in the controlled synthesis of ultra-high molecular weight polymers, polymerization-induced self-assembly, and biocompatible polymerizations [81].

Perspective: Semiconducting Nanomaterials Used as Photoinitiators/Photocatalysts during Photopolymerization
In recent years, semiconducting nanomaterials (SNMs) have been proven to be a potential substitution for metal complexes and organic PCs as photoinitiators/photocatalysts during photopolymerization due to their high extinction coefficients (>10 5 M −1 cm −1 ), broad absorption spectra, and multiple molecular binding points [82,83]. However, little attention has been paid to SNM-induced photopolymerization due to the broad gap between nanotechnology and polymerization science. In the previous literature, the SNMs have been proven to initiate polymerization by the generation of radical species from the co-initiators upon the application of light irradiation, and the proposed photoinitiation mechanisms of this are fully discussed by Zhu et al. [84]. In their review, the SNM-induced photopolymerization could be mainly divided into three possible categories: (A) A newly established photoinduced polymerization wherein the SNM serves as the photocatalysts to conduct a catalytic cycle as shown in Figure 10a. In this cycle, the active radicals can be generated via the direct reduction of the initiators (or polymer chain ends) by SNM during the polymerization process. Then, the radicals can propagate by transferring the electrons back to SNMs at the end of the photoinduced electron transfer process. (B) Photoinduced polymerization wherein the SNM serves as the photoactivators, donating excited electrons or holes to the co-initiators, e.g., tertiary amines, iodonium salts, and RAFT agents, etc., in the polymerization system, and provides the radical sources to initiate the monomers (See Figure 10b for the mechanism of this). (C) A photoinduced polymerization that is initiated by a radical species that is generated from the co-initiators; here, the SNMs act as photoinitiators to activate the co-initiators. According to different the photoinitiation mechanisms of SNMs which act as PIs, this kind of photopolymerization could be mainly divided into three possible pathways: (1) the direct photoreduction of the monomer via electron transfer from the SNMs' conduction band to the monomers with a proper band gap energy (see Figure 10c); (2) the direct oxidation of the monomer via hole transfer from the SNMs' valence band to the monomers with a proper band gap energy (see Figure 10d); (3) the initiation of polymerization via a charge transfer from the anion-localized surface of the SNMs to the monomers (see Figure 10e). Moreover, the use of SNMs as photoinitiators/photocatalysts without the use of a co-initiator during the polymerization process has become increasingly popular recently. Due to the aforementioned advantages of SNM, such as a high absorption coefficient and a tunable solubility, SNM-photoinduced polymer-ization gives new opportunities to expand the fields of photo-3D printing. As a perspective, the use of SNMs for photopolymerization in 3D printing could be achieved with a lower initiator/catalyst loading time, a higher conversion rate, the versatile functionalization of it, and it could even be performed in the aqueous phase.

Conclusions
According to the previous literature, numerous newly developed dye-based PISs following the Type II mechanisms exhibited efficient performances during light-induced polymerization, and as well as this, the attempts to explore the new mechanisms for photopolymerization following the Type I mechanism which were performed on RAFT, Photo-RAFT polymerized materials, Photoinitiator-RAFT polymerized materials, even performed in the aqueous phase, were successfully developed. Among these research studies, most of organic dye-based PISs and photochemical mechanisms are applicable in many applications, e.g., 3D printing and photocomposites, etc. To gain another perspective, the chemical modification of the existing organic dyes with a versatile functionalization to achieve a higher conversion rate for the acrylate monomer with a lower initiator/catalyst should be continued in the future. Furthermore, the SNMs with a high absorption coefficient and tunable solubility acting as photoinitiators/photocatalysts during the polymerization process provides new opportunities to expand the applications for photopolymerization, e.g., photo-3D printing. In conclusion, the photopolymerization has been proven to take an important place in 3D printing, and the molecular design of new photoinitiators/photocatalysts that are based on organic dyes can be regarded as an efficient bridge between the photopolymer materials and 3D printing orother technologies such as photolithography.

Conclusions
According to the previous literature, numerous newly developed dye-based PISs following the Type II mechanisms exhibited efficient performances during light-induced polymerization, and as well as this, the attempts to explore the new mechanisms for photopolymerization following the Type I mechanism which were performed on RAFT, Photo-RAFT polymerized materials, Photoinitiator-RAFT polymerized materials, even performed in the aqueous phase, were successfully developed. Among these research studies, most of organic dye-based PISs and photochemical mechanisms are applicable in many applications, e.g., 3D printing and photocomposites, etc. To gain another perspective, the chemical modification of the existing organic dyes with a versatile functionalization to achieve a higher conversion rate for the acrylate monomer with a lower initiator/catalyst should be continued in the future. Furthermore, the SNMs with a high absorption coefficient and tunable solubility acting as photoinitiators/photocatalysts during the polymerization process provides new opportunities to expand the applications for photopolymerization, e.g., photo-3D printing. In conclusion, the photopolymerization has been proven to take an important place in 3D printing, and the molecular design of new photoinitiators/photocatalysts that are based on organic dyes can be regarded as an efficient bridge between the photopolymer materials and 3D printing orother technologies such as photolithography.